Like this document? Why not share!

- An Introduction to Crystallography by Hassan Harraz 4320 views
- Raman and his legacy by Tathagat Ka... by quark the science... 306 views
- BT631-14-X-Ray_Crystallography_Crys... by Rajesh G 669 views
- Pencil portrait eyes by qb3m19ef 401 views
- Dancing tips for beginners by Mitesh Take 124 views
- How to draw spiderman for beginners by tainyaa 450 views

1,488

-1

-1

Published on

No Downloads

Total Views

1,488

On Slideshare

0

From Embeds

0

Number of Embeds

0

Shares

0

Downloads

0

Comments

0

Likes

1

No embeds

No notes for slide

- 1. Crystal Morphology and Crystal Symmetry 1 1.1 Brief Historical Introduction Crystals, with their plane faces, sharp angles, and color, have excited interest since the earliest times. Their color and decorative qualities are recorded in the Bible [1]: we need not start as far back as that, but will consider instead some of the highlights in the build-up of the science of Crystallography. The Swiss naturalist Conrad Gessner [2] observed in 1564 that “one crystal differs from another in its angles, and consequently in its ﬁgure,” and Pliny [3], Caesalpinus [4], and Buffon [5] also denied “the ﬁxity of crystals.” Niels Stensen, a Dane, also known as Nicolaus Steno [6], showed in 1669 that crystals of quartz, although of varying edge lengths, nevertheless preserved constant angles between corresponding faces, an observation that led, after further work, to the law of constant interfacial angles (q.v.), sometimes called Steno’s law. Some examples of Steno’s ﬁgures for quartz are shown in Fig. 1.1. Pliny referred to quartz as krustallos (Gk. krnstallos ¼ ice), believing it to be ice permanently congealed by intense cold: “rain-water and pure snow are needed for its formation.” In the same year, Bartholinus [7] published his work on the Iceland Spar modiﬁcation of calcium carbonate: he measured the interfacial angles (q.v.) of crystal fragments and found that “the (cleavage) fragments have the same shape as the original crystal.” Johannes Kepler, bestknown for his research inastronomy, worked sometime for Emperor Rudolph II of Austria, who was somewhat negligent in paying salaries. Kepler, who was without money with which to purchasea Christmas present for a friendin 1611, wrote a booklet entitled The Six-Cornered Snowﬂake [8], Fig. 1.2. He had noticed that snow crystals of whatever shape always exhibited sixfold symmetry. He speculated on a relationship between the snow crystal and a hexagonal close packing of spheres: he recognized the genre of crystal symmetry, which was to be developed about two centuries years later. Jokingly,hepassedoff his“NewYear’sGift”asamere“nothing” (like hisﬁnances),makinga playonthe word nix, which means “snowﬂake” in Latin but “nothing” in Lower German, Kepler’s language. Over the period 1688–1705, many investigations by the Italian physicist Giovanni Guglielmini [9] conﬁrmed and extended the work of Steno, and during 1772–1783, about a century after Steno, the Frenchman Jean-Baptiste Rome´ de l’Isle [10] carried out an extensive series of measurements that conﬁrmed fully Steno’s ﬁndings: he stated further, as a law, that “the interfacial angles of a crystal material are characteristic of it.” In his work, he made much use of the contact goniometer, developed by Arnould Carangeot [11], for measuring interfacial angles on crystals. His compatriot Rene´ Just (Abbe´) Ha€uy [12] published a treatise on mineralogy in 1801 in which he envisaged crystals built up by stacking identical blocks of structural material in ways that led to the shapes of crystals, thus explaining Steno’s law. He was led to this view by the observation that when M. Ladd and R. Palmer, Structure Determination by X-ray Crystallography: Analysis by X-rays and Neutrons, DOI 10.1007/978-1-4614-3954-7_1, # Springer Science+Business Media New York 2013 1
- 2. Fig. 1.1 Examples of Steno’s drawings of transverse sections of different crystal specimens of quartz, SiO2; the interfacial angles are 120 or (120/2) in each case Fig. 1.2 The cover (in translation) of Kepler’s booklet on The Six-Cornered Snowﬂake; some of Kepler’s many drawings of snowﬂakes appear on the cover (reproduced by courtesy of Paul Dry Books) 2 1 Crystal Morphology and Crystal Symmetry
- 3. crystals of calcite were broken, they always formed rhombohedral-shaped fragments whatever the shape of the original crystal, an observation similar to that made by Bartholinus. Other crystals cleaved into different shapes, such as cubes; Fig. 1.3 illustrates some of Ha€uy’s ﬁgures. He laid the foundation for the law of rational intercepts (q.v.), which demonstrated, albeit implicitly, a shape for the unit cell (q.v.) of a crystal. He described also different crystal shapes, or habits, obtained by the packing of different shaped blocks. In the period 1804–1815, the German scientists Christian Weiss [13] and Frederick Mohs [14], independently, identiﬁed the six “major” crystal systems (q.v.)—it seems that they did not distinguish between the two systems that we now recognize as trigonal and hexagonal. Another German scientist Johann Hessel [15] determined the 32 crystallographic point groups (q.v.) in 1835 and his compatriot Moritz Frankenheim [16] also described six crystal systems and, additionally, the 32 crystal classes in 1842. Crystal classes are names for the general forms (q.v.) of crystals, of which we shall have more to say later, Sect. 1.4.2; Fig. 1.4 illustrates two examples of crystal class. A next landmark was that contained in the work of William Miller, 1839, who proposed an unambiguous notation for specifying the orientations of the faces of a crystal, leading to the Miller Indices [17] (q.v.), based on the scalar equation of a plane; the law of rational indices is clear from Miller’s work—the descriptor “law of rational ratios of intercepts” is perhaps more apt. The regular arrangements of points in space were addressed by August Bravais [18] in 1846, who derived the 14 Bravais lattices. Actually, Frankenheim had derived 15 such lattices in 1842, but Bravais showed that two of them were identical. For his infelicity, Frankenheim’s name is frequently omitted from a discussion of lattices, albeit the nature of his 15th lattice was never completely clear. Continuing the development of crystal symmetry, we have at the end of the nineteenth century, Yevgraf Fyodorov [19] (in Russia), Artur Sch€onﬂies [20] (in Germany), and William Barlow [21] (in Britain), all independently, describing the 230 ordered spatial patterns, or space groups (q.v.), that represented the possible ways of arranging inﬁnite arrays of points (atoms) regularly in space, commensurate with the 14 Bravais lattices. By that time, the work of mineralogists and mathematicians had led to a well-deﬁned study of the external form (morphology) of crystals, as well as to predictions about their internal structure. The totality of mineralogical studies was collected in the extensive six-volume treatise ChemischeKris- tallographie of Paul von Groth, the ﬁrst part of which was published in 1904. The time was right for a major breakthrough, and we arrive at the year 1912 and the inception of the study of crystals by X-ray diffraction methods: X-ray Crystallography was born. Fig. 1.3 Examples of Ha€uy’s ﬁgures. (a) Rhombic dodecahedron formed from stacked cubes, as in garnet (idealized formula Ca3Al2Si3O12). (b) Pentagonal dodecahedron formed from stacked cubes, as in K2Mn2(SO4)3. (c) Scalenohe- dron formed from stacked rhombohedra, as in calcite, CaCO3 1.1 Brief Historical Introduction 3
- 4. The classic experiment [22], suggested by Laue,1 and performed by Paul Friedrich and Walter Knipping, demonstrated the diffraction of X-rays from a crystal of copper sulfate. This material was, perhaps, not the best choice because of its low (triclinic) symmetry. Nevertheless, the diffraction effects showed conclusively both that crystals were periodic in three dimensions and that X-rays possessed wave-like properties. Figure 1.5 shows X-ray diffraction patterns from early experiments on X-ray diffraction. The results from this work may be said to be a landmark in the development of modern science. The diffraction technique that was initiated by Laue was improved quickly by W. L. Bragg, in his work on crystals of the alkali-metal halides and other crystals. Barlow, one of those who had derived the space groups earlier, had also developed structure models for some metallic elements, and simple binary compounds such as sodium chloride, cesium chloride, and zinc blende. None of his results was proved at that time: all were speculative, but remarkably accurate, as it turned out. Bragg [23] investigated the X-ray diffraction patterns of sodium chloride and other alkali halides and zinc blende (ZnS). He found that the models suggested by Barlow were correct, and other models proposed by Barlow, such as cubic close-packed and hexagonal close-packed structures for metallic elements, were conﬁrmed. The number of structure analyses grew very rapidly: Fig. 1.6 is a stereo- view of the structure of sodium chloride, NaCl. Several stereoviews are used in this book in order to Fig. 1.4 Examples of crystal classes: (a) Rhombic disphenoid, showing left-hand and right-hand enantiomorphs (q.v.). (b) Hex(akis) octahedron 1 In 1913, Laue’s father was raised to the ranks of hereditary nobility; Laue then became von Laue. 4 1 Crystal Morphology and Crystal Symmetry
- 5. demonstrate clearly the three-dimensional nature of crystal structures, and Appendix A describes the process of stereoviewing, and the construction of a simple stereoviewer. The early structure analyses were carried out with the aid of an X-ray ionization spectrometer, the forerunner of the modern single-crystal X-ray diffractometer, designed largely by W. H. Bragg [24]. Generally, the name Bragg refers to W. L. Bragg, but his father (W. H.) also played a highly signiﬁcant role at the very beginning of the technique of crystal structure analysis by X-ray diffraction. X-ray diffraction provides the most powerful technique for probing the internal structures of crystals and for determining with high precision the actual atomic arrangement in space. Figure 1.7 shows a three-dimensional contour map of the electron density in a medium-sized molecule, euphenyl iodoace- tate [25], C32H53O2I. The contour lines join points of equal electron density in the structure; hydrogen atoms are not revealed in this map because of their relatively small scattering power for X-rays. If we assume that the centers of atoms are located at the maxima in the electron density map, we can deduce the molecular model in Fig. 1.8a; the chemical structural formula is shown for comparison in Fig. 1.8b. The iodine atom is represented by the large number of contours at the extreme left of Fig. 1.7. The carbon and oxygen atoms are depicted by approximately equal numbers of contours. The atoms in the side chain, shown on the extreme right of the ﬁgure, have contours that are spaced further apart. Thermal Fig. 1.6 Stereoview of the face-centered cubic unit cell and its environs for the crystal structure of sodium chloride: ¼ ClÀ , ¼ Naþ Fig. 1.5 The ﬁrst X-ray diffraction photograph by Friedrich et al. [22]. (a) Copper sulfate pentahydrate, CuSO4·5H2O, showing no symmetry. (b) Zinc blende (the ﬁrst crystal structure to be fully determined), ZnS, showing fourfold symmetry (Bragg WH, Bragg WL (1949) The crystalline state, vol 1. G. Bell and Sons) 1.1 Brief Historical Introduction 5
- 6. vibrationsof the atoms are mostsevere in this portion ofthemolecule, andtheyhavethe effect of smearing out the electron density, so that its gradient, represented by the closeness of the contours, is less steep than in other parts of the molecule. Molecules of much greater complexity than that in this example are now being investigated; the structures of proteins, enzymes, and nucleic acids—the “elements” of life itself—are being revealed by powerful X-ray diffraction techniques [25a]. Fig. 1.8 Euphenyl iodoacetate, C32H53O2I. (a) Molecular model, excluding hydrogen atoms. (b) Chemical structural formula: the orientations at carbon atoms 13, 14, and 17 are a, b, and a, respectively (standard numbering) Fig. 1.7 Three-dimensional electron density contour map for euphenyl iodoacetate, as seen along the b direction of the unit cell; the contours connect points of equal electron density: the electron density contours have been drawn on a set of perspex sheets and stacked normal to b 6 1 Crystal Morphology and Crystal Symmetry
- 7. 1.2 The Crystalline State A crystalline substance may be deﬁned as a homogeneous solid having an ordered internal atomic arrangement2 and a deﬁnite overall chemical composition, albeit non-stoichiometric in some exam- ples. In addition to the more obvious manifestations of crystalline materials, like sugar and common salt, other substances, such as cellophane sheet and ﬁbrous asbestos, which reveal different degrees of long-range order (extending over many atomic dimensions), may be described as crystalline. With the unaided eye, fragments of glass and of quartz look similar to each other, yet quartz is crystalline andglassisnon-crystalline,oramorphous.Glass hasanatomicarrangement thatdisplaysonly very short-range order (extending over a few atomic dimensions). Figure 1.9 illustrates the structures of quartz and silica glass; both of them are based on the same atomic group, the tetrahedral SiO4 structural unit, but in quartz these groups are arranged regularly throughout three-dimensional space. A crystal may be deﬁned as a substance that is crystalline and periodic in three dimensions and bounded by plane faces. We have now made the useful distinction that crystalline substances exhibit long-range order in three dimensions or less, whereas crystals have both this three-dimensional regularity and plane bounding faces; see also Sect. 1.4.3. 1.2.1 Crystallographic Reference Axes In describing the external features of crystals, we make use of relationships in coordinate geometry. It is important to set up a system of reference axes, and three such axes are needed in the description of a crystal, Fig. 1.10. By convention, the x, y, and z crystallographic reference axes are set parallel to important directions in the crystal. We shall see later that these directions (crystal edges, or possible crystal edges) are related closely to the symmetry of the crystal; in some cases, a choice of non- orthogonal axes then will arise naturally. It is usual to work with right-handed axes. In Fig. 1.11, +y and +z are in the plane of the paper, as shown, and +x is directed forward; the succession +x ! +y ! +z simulates an anticlockwise screw motion, which is one way of describing right-handed axes. Notice the selection of the interaxial angles a, b, and g and the mnemonic connection between their positions and the directions of the x, y, and z axes. 1.2.2 Equation of a Plane The plane ABC shown in Fig. 1.12 intercepts the x, y, and z axes (which need not be orthogonal) at A, B, and C, respectively. ON is the perpendicular from the origin O to the plane; it has the length d, and its direction cosines (see Web Appendix WA1) are cos w, cos C, and cos o with respect to OA, OB, and OC, respectively, which have the lengths a, b, and c, and P is any point X, Y, Z in the plane ABC. Let PK be parallel to OC and meet the plane AOB at K, and let KM be parallel to OB and meet OA at M. Then the lengths of OM, MK, and KP are X, Y, and Z, respectively. Since ON is the projection of OP on to ON, it is equal to the sum of the projections OM, MK, and KP all on to ON. Hence, d ¼ X cos w þ Y cos C þ Z cos o (1.1) 2 See also Sect. 8.9. 1.2 The Crystalline State 7
- 8. In DOAN, d ¼ OA cos w ¼ a cos w. Similarly, d ¼ b cos C ¼ c cos o; dividing by d: ðX=aÞ þ ðY=bÞ þ ðZ=cÞ ¼ 1 (1.2) Equation (1.2) is the intercept form of the equation of the plane ABC. 1.2.3 Indices of Planes and the Law of Rational Intercepts Miller Indices The faces of a crystal are planes in three-dimensional space. Once the crystallographic axes are chosen, a parametral plane may be deﬁned and any other plane described by reference to it in terms of three numbers h, k, and l. If the parametral plane is designated by integral values of h, k, and l, Fig. 1.9 Arrangements of SiO4 structural units (the darker spheres represent Si). (a) a-Quartz. (b) Silica glass (reproduced by courtesy of NPL) 8 1 Crystal Morphology and Crystal Symmetry
- 9. normally (111), then the indices of all other crystal faces are small integer values, rarely more than 5. This result is known as the law of rational intercepts (indices) (q.v.) and has a basis in lattice theory. A notation for describing the faces of a crystal was introduced ﬁrst by William Whewell in 1825 and developed fully by Miller [17] in 1839, and h, k, and l are the Miller indices. In Fig. 1.13, let the parametral plane (111) be ABC, making intercepts a, b, and c on the crystallographic axes x, y, and z, respectively. Another plane LMN makes corresponding intercepts of lengths a/h, b/k, and c/l. The Miller indices of plane LMN are expressed by the ratios of the intercepts of the parametral plane to those of the plane LMN. If in the ﬁgure, a/h ¼ a/4, b/k ¼ b/3, and c/l ¼ c/2, then LMN is (432), see also Sect. 2.3. If fractions occur in formulating h, k, or l, they are Fig. 1.11 Right-handed, general crystallographic axes x, y, and z, and the interaxial angles a, b, and g Fig. 1.10 Idealized tetragonal crystal with orthogonal (mutually perpendicular) axes x, y, and z drawn in 1.2 The Crystalline State 9
- 10. cleared by multiplication throughout by the lowest common denominator. Conditions of parallelism to axes and intercepts on the negative sides of the axes lead respectively to zero or negative values for h, k, and l. Thus, ABDE is the plane (110), BDFG is (010), and PBQ is ð213Þ.3 It may be noted that it has not been necessary to assign numerical values to either a, b, and c or a, b, and g in order to describe the crystal faces by their Miller indices. In the next chapter, we shall identify a, b, and c with the edges of the crystal unit cell in a lattice, but this relationship is not needed at present. The preferred choice of the parametral plane leads to small numerical values for the Miller indices of crystal faces. If LMN had been chosen as (111), then ABC would have been (346). Summarizing, we may say that the plane (hkl) makes intercepts a/h, b/k, and c/l along the crystallographic x, y, and z axes, respectively, where a, b, and c are the corresponding intercepts made by the parametral plane. The conventional choice of reference axes leads to special relationships between the intercepts a, b, c, and the (111) parametral plane, and between the interaxial angles a, b and g, in all crystals other than triclinic (q.v.). From (1.1) and (1.2), the intercept equation of the general plane (hkl) may be written as ðhX=aÞ þ ðkY=bÞ þ ðlZ=cÞ ¼ 1 (1.3) The equation of the parallel plane passing through the origin is ðhX=aÞ þ ðkY=bÞ þ ðlZ=cÞ ¼ 0 (1.4) it must satisfy the condition X ¼ Y ¼ Z ¼ 0. It follows from (1.4) that the Miller indices of a crystal plane cannot be determined if the origin is chosen on that plane. Fig. 1.12 Plane ABC in three-dimensional space; ON, of length d, is the normal to the plane from the origin O 3 Read as “bar-two one bar-three,” or “two-bar one three-bar” in the USA. 10 1 Crystal Morphology and Crystal Symmetry
- 11. Miller–Bravais Indices In crystals that exhibit sixfold or threefold symmetry referred to hexagonal axes, see Table 1.3, four axes of reference may be used, an extension of the Miller indices due to Bravais [18]. The axes are designated x, y, u, and z; the x, y, and u axes lie in one plane, at 120 to one another, and the z axis is perpendicular to the x, y, u plane, Fig. 1.14; the sequence x, y, u, z is right-handed. Planes in these crystals are described by four numbers, the Miller–Bravais indices h, k, i, and l. The index i is not Fig. 1.13 Miller indices of planes: OA ¼ a, OB ¼ b, OC ¼ c; ABC is the parametral plane (111), and LMN is the plane (hkl) Fig. 1.14 Miller–Bravais indices (hkil). The crystallographic axes are labeled x, y, u, z, and the plane ð2354Þ is shown; the parametral plane is ð1121Þ 1.2 The Crystalline State 11
- 12. independent of h and k: thus, if the plane ABC in Fig. 1.14 intercepts the x and y axes at a/2 and b/3, for example, then the u axis is intercepted at Àu/5. If also the z axis is intercepted at c/4, then the plane is designated ð2354Þ. From Problem 1.14, we show that, in general, i ¼ À(h + k). Law of Rational Intercepts Planes that appear as external crystal faces are those most densely populated by the units of structure. Consider a P orthorhombic lattice, Fig. 2.4. The (010) planes are more densely populated in proportion to 1/ac than are the (110) planes at 1=ðc ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 þ b2 p Þ which, in turn, are more densely populated than, say, the (210) at 1=ðc ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 þ 4b2 p Þ. The more densely populated planes are those of wider spacing in a given material: d is proportional to the reticular density or to 1/reticular area. The planes with the lower values of S2 , where S2 ¼ h2 + k2 + l2 , lead to the more stable (lower energy) crystal state. If we consider a cubic crystal, for example, then d ¼ a=ðh2 þ k2 þ l2 Þ1=2 ¼ a=S, from Table 2.4, so that for the three cubic lattices, Fig. 2.4, we have: P hkl 100 110 111 210 211 221 S2 1 2 3 5 6 9 Showing a preference for hexahedral {100} forms, as in caesium chloride or sodium chlorate. I hkl 110 200 211 310 420 442 S2 2 4 6 10 20 36 Showing a preference for dodecahedral {110} forms, as in garnet structures. F hkl 111 200 220 310 420 422 S2 3 4 8 10 20 246 Showing a preference for octahedral {111} forms, as in diamond and calcium ﬂuoride. Thus, on grounds of stability, planes of larger d-values (smaller values of h, k, and l) are to be expected. 1.2.4 Axial Ratios If both sides of (1.4) are multiplied by b, we obtain hX a=b þ kY þ lZ c=b ¼ 0 (1.5) The quantities a/b and c/b are termed axial ratios; they can be deduced from an analysis of the crystal morphology, but not the individual values of a, b, or c. 1.2.5 Zones Most well formed crystals have their faces arranged in groups of two or more with respect to certain directions in the crystal. In other words, crystals exhibit symmetry; this feature is an external manifestation of the ordered arrangement of atoms in the crystal. Figure 1.15 illustrates zircon, 12 1 Crystal Morphology and Crystal Symmetry
- 13. ZrSiO4, an example of a highly symmetric crystal. It is evident that several faces have a given direction in common. Such faces are said to lie in a zone, and the common direction is called a zone axis. Any two faces, (h1k1l1) and (h2k2l2), deﬁne a zone. The zone axis is the line of intersection of the two planes and is given by the solution of the equations ðh1X=aÞ þ ðk1Y=bÞ þ ðl1Z=cÞ ¼ 0 ðh2X=aÞ þ ðk2Y=bÞ þ ðl2Z=cÞ ¼ 0 (1.6) for the two planes passing through the origin (since we are concerned here only with the directional- ity). The solution is given by the line X aðk1l2 À k2l1Þ ¼ Y bðl1h2 À l2h1Þ ¼ Z cðh1k2 À h2k1Þ (1.7) which must also pass through the origin. It may be written as X=ðaUÞ ¼ Y=ðbVÞ ¼ Z=ðcWÞ (1.8) where [UVW] is called the zone symbol. If any other face (hkl) lies in the same zone as that deﬁned by (h1k1l1) and (h2k2l2), then it follows from immediately from (1.4) and (1.8), that hU þ kV þ lW ¼ 0 (1.9) which is an expression of the Weiss zone law [13]. For if planes (h1k1l1), (h2k2l2), and (hkl) lie in one and the same zone (tautozonal), then applying (1.6) to (hkl) and using (1.8) in the result leads to (1.9). We shall show this result in another way in Sect. 2.5.4. Fig. 1.15 A highly symmetric crystal (zircon, ZrSiO4), showing the Miller indices of some of its faces. What are the Miller indices of the other faces on this crystal? 1.2 The Crystalline State 13
- 14. In the zircon crystal, the vertical (prism) faces lie in one zone. If the prism faces are indexed in the usual manner, as in Fig. 1.15, then, from (1.7) and (1.8), the corresponding zone symbol is [001]. The symbols [UVW] and ½ U V W refer to lines that are collinear, but of opposite sense. From (1.9), we see that (110) and (100) are faces in the [001] zone, but (111) is not. Other relationships follow from (1.9) in a similar way. In the manipulation of these equations, it may be noted that a zone axis is described by [UVW], the simplest symbol; the axes that may be described as [nU, nV, nW] (n ¼ 0, Æ1, Æ2,. . .) are coincident with [UVW] in crystal morphology. From (1.6), a zone symbol cannot be determined from two faces (hkl) and ðh k lÞ. Thus, although both the (110) and ð110Þ planes lie in the [001] zone, this zone symbol could not be determined from these two planes alone. Angle Between Two Directions (Zone Axes) The angle y between two directions [UVW] and ½U0 V0 W0 is given by y ¼ r½UVW Á r½U0V0W0 r½UVWr½U0V0W0 (1.10) the evaluation of which follows from (2.16). Fig. 1.16 Optical goniometry. (a) Principle of the reﬂecting goniometer; AB and BC represent two adjacent tautozonal faces on the crystal. (b) Two-circle optical goniometer; the crystal rotates about the vertical circle (the zone axis through O), and the telescope and collimator rotate about the horizontal circle 14 1 Crystal Morphology and Crystal Symmetry
- 15. Constancy of Interfacial Angles The law of constant interfacial angles states that in all crystals of the same substance, angles between corresponding faces have a constant value. Interfacial angles may be measured by a goniometer, the ﬁrst of which was that developed by Carangeot [11], as we noted earlier. The principle of the more precise reﬂecting goniometer is shown in Fig. 1.16a, which forms the basis of modern optical goniometry. A crystal is arranged to rotate about a zone axis O, which is set perpendicular to a plane containing the incident and crystal-reﬂected light beams. Parallel light reﬂected from the face AB is received by a telescope. If the crystal is rotated in a clockwise direction, a reﬂection from the face BC is received next when the crystal has been turned through the angle F; then, the interfacial angle is 180 À F . Accurate goniometry brought a quantitative signiﬁcance to observable angular relationships in crystals. Figure 1.16b illustrates a simple two-circle optical goniometer. 1.3 Stereographic Projection: Brief Survey A representation of the many faces of a crystal by means of a convenient two-dimensional illustration may be achieved by means of a stereographic projection, or stereogram. Figure 1.17 shows a cubic crystal set within a sphere of arbitrary radius, with the normals to the sets of crystal faces drawn to intersect the sphere. Lines are drawn from the intersections with the sphere to meet the horizontal plane, or primitive, which becomes the plane of projection. An intersection from the upper hemi- sphere on to the horizontal plane, a pole, is marked as ● and that from the lower hemisphere as ○; where the two coincide the notation used is the dot inside the circle. Thus, we obtain Fig. 1.18, which may be indexed for the given crystal as shown in Fig. 1.19. Later in this chapter, we shall introduce a modiﬁcation for the notation of points on a stereogram, for reasons that will be there described. Fig. 1.17 Spherical projection of the cubic crystal showing three forms of planes: cube—faces b, e, d, and parallel faces; octahedron—faces r, m, n, q, and parallel faces; rhombic dodecahedron— faces f, g, p, o, c, a, and parallel faces. The x, y, and z axes are chosen parallel to important (symmetry) directions in the crystal; the radius of the sphere is arbitrary. The inclined great circle, b, m, o0 , q0 ,. . ., projects as G3G0 3 in Fig. 1.18 1.3 Stereographic Projection: Brief Survey 15
- 16. Fig. 1.18 Stereogram of the crystal shown in Fig. 1.17; the zone circle (great circle) G1G0 1, symbol [101], passes through e, q, a, n, e0 , q0 , a0 , n0 ; the zone circle G2G0 2 symbol ½110, passes through f, r, d, q0 , f0 , r0 , d0 , q; the zone circle G3G0 3, symbol [011], passes through b, m, o0 , q0 , b0 , m0 , o, q Fig. 1.19 Stereogram in Fig. 1.18 indexed, taking r as 111. The zone containing (100) and (111) is ½011, and that containing (010) and (001) is [100]. From (1.7), (1.8), and (1.9), it follows that the face p common to these two zones is (011) 16 1 Crystal Morphology and Crystal Symmetry
- 17. The important feature of the stereogram for our purposes is that it preserves the interfacial angles of the crystal and, hence, displays faithfully the crystal symmetry. A more detailed description of the stereographic projection may be found in the Web Appendix WA2. 1.4 External Symmetry of Crystals The existence of faces on a crystal in groups of two or more, in a similar orientation with respect to some line or plane in the crystal, is a manifestation of symmetry. The crystal drawing of zircon in Fig. 1.15 shows several sets of symmetrically arranged faces. Few of us have difﬁculty in recognizing symmetry in two-dimensional pictures of objects such as a dumbbell, the three-legged emblem of the Isle of Man, a Maltese cross, the ﬁve-petal Tudor rose, the six-pointed Star of David; see Problem 1.10(c). But it is a rather different matter when we are dealing with three-dimensional objects. The problem arises ﬁrst from the fact that we can see all parts of a two-dimensional object simultaneously, and thus we take in the relation of the parts to the whole; but we cannot do that so easily with three-dimensional objects. Secondly, while some three-dimensional objects, such as ﬂowers, pencils, and architectural columns, are simple enough for us to visualize and to rotate in our mind’s eye, few of us have a natural gift for mentally perceiving and manipulating more complex three-dimensional objects. Nevertheless, the art of doing so can be developed with suitable aids and patience. If, initially, you have problems, take heart. You are not alone and, like many before you, you will be surprised at how swiftly the required facility can be acquired. Engineers, architects, and sculptors may be blessed with a natural three-dimensional visualization aptitude, but they have learned to develop it—particularly by making and handling models. Standard practice in the past was to reduce three-dimensional objects to one or more two-dimensional drawings (projections and elevations): it was cheap, well suited to reproduction in books, and less cumbersome than handling three-dimensional models. In this book, we shall continue to use such two- dimensional representations where appropriate, but to rely on them exclusively only delays the acquisi- tion of a three-dimensional visualization ability. Fortunately, we can now use stereoscopic image pairs, such as that shown in Fig. 1.6. These illustrations are a great help, but, because they provide a view from only one standpoint, they are not always quite the equal of models that can be examined by hand. Symmetry Symmetrymaybe deﬁned as thatspatial property of abody(or pattern) by whichthebody (orpattern) can be brought from an initial state to another indistinguishable state by means of a certain operation—a symmetry operation. For our purposes, the operation will be considered to take place in n-dimensional space (n ¼ 1, 2, or 3) and to represent an action with respect to a symmetry element. Symmetry Elements and Symmetry Operations A symmetry element is a geometrical entity (point, line, or plane) in a body or assemblage, with which is associated an appropriate symmetry operation. The symmetry element is strictly conceptual, but it is convenient to accord it a sense of reality. The symmetry element connects all parts of the body or assemblage as a number of symmetrically related parts. The term assemblage is often useful because it describes more obviously a bundle of radiating face normals, Fig. 1.17, or a number of bonds emanating from a central atom in the case of a molecule or ion, Fig. 1.34, to which these symmetry concepts equally apply. The symmetry operation corresponding to a symmetry element, when applied to a body, converts it to a state that is indistinguishable from the initial state of that body, and thus the operation reveals 1.4 External Symmetry of Crystals 17
- 18. the symmetry inherent in the body. In many cases, different symmetry operations can reveal one and the same symmetry element. Thus, 31 (¼3), 32 , and 33 (¼3) may be regarded as either multiple steps of 3, a threefold operation (q.v.), or single-step operations in their own, but all are contained within the same single symmetry element, 3. The latter idea is of particular importance in the study of group theory. Symmetry elements may occur singly in a body, as in Fig. 1.20, for example, or in certain combinations, as in the example of Fig. 1.22. Point Groups A set of interacting symmetry operations in a ﬁnite body, or just one such element, is referred to as a point group. A point group may be deﬁned as a set of symmetry operations the action of which leaves at least one point unmoved: this point is taken as the origin of the reference axes for the body, through which all symmetry elements pass. The assembly of points deﬁning a rotation axis or a mirror plane is effectively unmoved by their operations. It can be contended that, in real objects, since they are imperfect, even if only on a microscopic scale, an indistinguishable second state can be obtained only by a rotation of 360 (or 0 ); this operation is identity, or “doing nothing.” For practical purposes, however, the effects of most Fig. 1.20 Some two-dimensional objects and their point-group symbols. The motifs are built up from the asymmetric unit (a), by operating on it according to the point-group symmetry. Note that, except in (a), the symmetry element intersects the asymmetric unit and lies at the center of each ﬁgure 18 1 Crystal Morphology and Crystal Symmetry
- 19. imperfections are small, and although our discussion of symmetry will be set up in terms of ideal geometrical objects, the extension of the results to real situations is scientiﬁcally rewarding. The observable symmetry may depend upon the nature of the examining probe, and different results for a given material may arise in terms of its optical, magnetic, and photoelastic properties, and from neutron diffraction, Sect. 11.1. Here, we shall be concerned with the symmetry shown by directions in space, such as the normals to the faces on crystals, or the bond directions in chemical species. Such angular relationships can be presented conveniently on stereograms, Sect. 1.3, and we shall draw fully on this method of representation in the ensuing discussion. Several concepts in symmetry can be introduced conveniently with two-dimensional objects; subsequently, the third dimension can be introduced mainly as a geometrical extension of the two- dimensional ideas. There is a single one-dimensional point group; it is more difﬁcult to grasp conceptually, and we shall not be particularly concerned with it in this book. 1.4.1 Two-Dimensional Point Groups “We proceeded straight from plane geometry to solid bodies in motion without considering solid bodies ﬁrst on their own. The right thing is to proceed from second dimension to third, which brings us Fig. 1.21 Stereograms of the point groups of the objects in Fig. 1.20; the conventional graphic symbols for R (R ¼ 1, 2, 3, 4, 6) and m are shown 1.4 External Symmetry of Crystals 19
- 20. Fig. 1.22 Further two-dimensional objects with their stereograms and point groups. (a) 2mm. (b) 3m. (c) 4mm. (d) 6mm 20 1 Crystal Morphology and Crystal Symmetry
- 21. to cubes and other three-dimensional ﬁgures” [26]. If we examine the two-dimensional objects in Fig. 1.20, we can discover two types of symmetry elements that can bring an object from one state to another indistinguishable state: parts (a) to (e) of Fig. 1.20 depict rotational symmetry, whereas (f) shows reﬂection symmetry. Rotation Symmetry A two-dimensional objectpossessesrotationalsymmetry of degree R (or R-foldsymmetry) abouta point if it can be brought from one state to another indistinguishable state by each and every rotation of (360/R) about that symmetry point. Figure 1.20a–e illustrate the rotational symmetry elements R equal to 1, 2, 3, 4, and 6, respectively. The onefold element is the identity element and is crystallographically trivial; every object has onefold symmetry. Reﬂection Symmetry A two-dimensional object possesses reﬂection symmetry, symbol m, if it can be brought from one state to another indistinguishable state by reﬂection across the symmetry line. The operation is not one that we can perform physically with an object, unlike rotation, but we can appreciate from the object itself (and its stereogram) that m symmetry is present. The m line divides the ﬁgure into its asymmetric unit, , and a mirror image or enantiomorph of this unit, , which situation (left- hand–right-hand relationship) is characteristic of reﬂection symmetry, Fig. 1.20f. Each of the objects in Fig. 1.20 has a symmetry pattern that can be described by a two-dimensional point group, and it is convenient to illustrate these point groups by stereograms. Figure 1.21 shows stereograms for the two-dimensional point groups 1, 2, 3, 4, 6, and m. It should be noted that in using stereogram-like drawings to illustrate two-dimensional symmetry, the representative points (poles) must fall on the perimeter; such situations may represent special forms (q.v.) on the stereograms of three-dimensional objects. Combinations of R and m lead to four more point groups; they are illustrated in Fig. 1.22. We have deliberatelyomittedpointgroupsinwhichR ¼ 5 andR ! 7,for a reasonthat willbediscussedinChap.2. It is convenient to allocate the ten two- dimensional point groups to two-dimensional systems and to choose reference axes for the objects in close relation to the directions of their symmetry elements. Table 1.1 lists these systems, together with the meanings of the positions in the point-group symbols. It should be noted that combinations of m with R (R 2) introduce additional reﬂection lines of a different crystallographic form. In the case of 3m, however, these additional m lines are coincident with the ﬁrst set; the symbol 3mm is not meaningful. Table 1.1 Two-dimensional point groups and notation Symbol meaning, appropriate to position occupied System Point groups First position Second position Third position Oblique 1, 2 Rotation about a point – – Rectangular 1ma As above m ⊥ x – 2mm As above m ⊥ x m ⊥ y Square As above – – 4mm As above m ⊥ x, y m at 45 to x, y Hexagonal 3 As above – – 3m As above m ⊥ x, y, u – 6 As above – – 6mm As above m ⊥ x, y, u m at 30 to x, y, u a Usually written as m, but the full symbol is given here in order to clarify the positions of the symmetry elements in the symbol 1.4 External Symmetry of Crystals 21
- 22. It is important to remember the relative orientations of the symmetry elements in the point groups and the variations in the meanings of the positions in the different systems. In the two-dimensional hexagonal system, three axes may be chosen in the x, y plane; this selection corresponds with the use of Miller–Bravais indices in three dimensions. 1.4.2 Three-Dimensional Point Groups The symmetry elements encountered in three dimensions are rotation axes (R), inversion axes (R), and a reﬂection (mirror) plane (m). A center of symmetry can be present also, although this symmetry element may be included in a point group that contains the element R, as we shall see, and a check for this must be made. The operations of rotation and reﬂection are similar to those in two dimensions, except that the geometric extensions of the operations are now increased to rotation about a line and reﬂection across a plane, respectively. Inversion Axes An object is said to possess an inversion (strictly, roto-inversion) axis4 R if it can be brought from one state to another indistinguishable state by the combined actions of rotation by (360/R) about the axis and inversion through a point on the axis that also serves as the origin point; the two actions comprise a single symmetry operation. Like mirror symmetry, Sect. 1.4.1, the inversion axis is a physically non-performable symmetry operation on a model, but it may be represented conveniently on a stereogram. It is a little more difﬁcult to envisage this operation than those of rotation and reﬂection. Figure 1.23 illustrates a hypothetical molecule having a vertical 4 axis: the stereoscopic effect can be created by using a stereoviewer (see Appendix A for instructions for making a model with 4 symmetry). In crystals, R in R, can take only the values 1, 2, 3, 4, and 6; this is sometimes referred to as the crystallograpic restriction theorem. A simple explanation for this restriction is that only ﬁgures that are based on these rotational symmetries can be stacked together to ﬁll space completely in a periodic manner, as Fig. 1.27 shows; see also Sect. 1.4.3. A further discussion of these restrictions on R is given in Sect. 2.6. In pictorial representations of the three-dimensional point groups, it is helpful to indicate the third dimension on their stereograms and, in addition, to illustrate the change-of-hand relationship that Fig. 1.23 Stereoview of a hypothetical C4 molecule; the 4 axis is in the vertical direction 4 Read as “bar-R”, or “R-bar” in the United States. 22 1 Crystal Morphology and Crystal Symmetry
- 23. occurs with R (including m) symmetry operations. For example, referring to Fig. 1.24, the element 2 lying in the plane of projection and the element 4 normal to the plane of projection, when acting on a point derived from the upper hemisphere (symbol ●), both move the point into the lower hemisphere region (symbol O). Both operations involve a reversal of the sign of the vertical coordinate, but only 4 involves also a change of hand, and this distinction is not clear from the conventional stereogram notation. Consequently, we shall adopt a symbolism, shown in Fig. 1.25, that is common to three- dimensional space groups, and which will affect the necessary distinction. With the modiﬁed notation, a representative point in the upper, l-positive hemisphere will now be shown by O+ , signifying, for example, the face (hkl), or its pole. A change of hemisphere to ðhklÞ will be indicated by OÀ , and a change-of-hand on reﬂection or inversion by or Fig. 1.25. This notation may appear to nullify partially the purpose of a stereogram. However, although the stereogram is a two-dimensional diagram, it is helpful here to convey a three-dimensional impression clearly, and this notation is used as an aid to this end. Figure 1.26a shows a stereogram for point group m. The inverse diad ð2Þ is lying normal to the m plane. A consideration of the two operations in the given relative orientations shows that they produce equivalent actions. It is conventional to use the symbol m for this operation, although sometimes it is helpful to employ the symbol 2 instead; potassium tetrathionate, Fig. 1.26b, crystallizes in point group m. Fig. 1.24 Stereograms of general forms. (a) Point group 2 (axis horizontal and in the plane of the stereogram). (b) Point group 4 (axis normal to the plane of the stereogram). In (a), the point ● is rotated through 180 to O: (1) and (2). In (b), the point ● is rotated through 90 and then inverted through the origin to O; this combined operation generates, in all, four symmetry-equivalent points: (1) ! (4) ! (3) ! (2) Fig. 1.25 (a) Stereograms from Fig. 1.24 in the revised notation: the different natures of points (2) in (a) and (2) and (4) in (b), all with respect to point (1), are now clear 1.4 External Symmetry of Crystals 23
- 24. We shall not be concerned here to derive the crystallographic point groups—and there are several ways in which it can be done5 —but to give, instead, a scheme which allows them to be worked through simply and adequately for present purposes. In addition, the program EULR, Sect. 13.2, shows how the combinations of symmetry operations based on R and R (R ¼ 1, 2, 3, 4 and 6) lead inter alia to the 32 crystallographic point groups. The symbols for rotation and reﬂection symmetry in three dimensions are similar to those already discussed; certain additional symbols are now required, and Table 1.2 lists them all. Crystal Classes There are 32 crystal classes that describe the possible types of crystals that occur. Each class has a name that corresponds to the general form on the crystal, and each class is characterized by a point group. A crystal form is the set {hkl} of faces (hkl) related by the point group of the crystal: if it is “general” then none of the (hkl) faces lies on symmetry elements; if it is a special form, then the faces of the set lie on symmetry elements. Two crystal classes were illustrated in Fig. 1.4: the rhombic disphenoid class (a) belongs to the orthorhombic system (to be discussed next) and shows point group 222; it has four similar scalene triangle faces and can exist in enantiomorphic forms. An example is Mozartite, CaMn(SiO4)(OH), which was ﬁrst noted in 1991, the 200th anniversary of the death of Mozart. Another, less exotic, example is Epsomite, MgSO4·7H2O. The hexakisoctohedron (cl. Gk. hexakis—six times; aka hexoctahedron) of class (b) belongs to the cubic system with point group m3m and is exhibited by some specimens of native silver; each face is a regular octahedron sub-divided into six equal triangular faces. Crystal Systems and Point-Group Scheme Crystals are grouped into seven systems according to the characteristic symmetry listed in Table 1.3. The characteristic symmetry refers to that minimum necessary for classiﬁcation of a crystal in a given system; a crystal of a given system may contain more than its characteristic symmetry. Fig. 1.26 Point group m. (a) Stereogram showing equivalence of m and 2 (the graphic symbol used here for 2 is useful, albeit not conventional). (b) Crystal of potassium tetrathionate (K2S4O6), point group m 5 See Bibliography (Ladd 1989). 24 1 Crystal Morphology and Crystal Symmetry
- 25. Fig. 1.27 Sections of three-dimensional ﬁgures and the rotational symmetries of their smallest structural units; (a–d) Space-ﬁlling patterns. In (e) and (f) the v-marks represent voids in the pattern (see also Problem 1.10a) Table 1.2 Three-dimensional symmetry symbols Symbol Name Action for indistinguishability Graphic symbol 1 Monad 360 (0 ) rotation; identity None 2 Diad 180 rotation projection, projection 3 Triad 120 rotation or inclined to projection 4 Tetrad 90 rotation projection, projection 6 Hexad 60 rotation projection 1 Inverse monad Inversiona 3 Inverse triad 120 rotation + inversion or inclined to projection 4 Inverse tetrad 90 rotation + inversion projection, projection 6 Inverse hexad 60 rotation + inversion projection m Mirror planeb Reﬂection across plane projection, projection a R is equivalent to R plus 1 only where R is an odd number: 1 represents the center of symmetry, but 2, 4, and 6 are not centrosymmetric point groups. For R even, R þ 1 R=m b The symmetry elements m and 2 produce an equivalent operation, with 2 oriented perpendicularly to the mirror plane
- 26. A crystallographic point-group scheme is given in Table 1.4, under the seven crystal systems as headings. The main difﬁculty in understanding point groups lies not so much in knowing the action of the individual symmetry elements, but in appreciating both the relative orientation of the different elements in a point-group symbol and the fact that this orientation changes among the crystal systems according to the principal symmetry axis, that is, the rotation axis R of highest degree. These orientations need to be learned: they form the key to point-group and space-group studies. Table 1.5 lists the meanings of the three positions in the three-dimensional point-group symbols. Tables 1.4 and 1.5 should be studied carefully in conjunction with Fig. 1.32. For example, consider carefully point groups 222 and 422, and note how and why the orientations repre- sented by the three positions in the symbol change their meanings. In 222, the three symmetry axes are along x, y, and z, respectively. In 422, 4 is taken along z, by convention; the ﬁrst symbol 2 (second position in the symbol) represents both the x and y directions, because they are equivalent under fourfold symmetry. This combination of 4 and 2 introduces symmetry along [110] and ½110, so that the second symbol 2 represents this symmetry. Similar situations exist among other point groups where the principal symmetry axis is of degree greater than 2. The reader should not be discouraged by the wealth of convention which surrounds this part of the subject. It arises for two main reasons. First, there are many different, equally correct ways of describing crystal geometry. For example, the unique axis in the monoclinic system could be chosen as x or z instead of y, or along some arbitrary direction. Secondly, a strict system of notation is Table 1.3 Crystal systems and their characteristics System Characteristic symmetry axes, with their orientation Parametral plane intercepts and interaxial angles, assuming the simplest indexing of facesa,b Triclinic None a 6C b 6C c; a 6C b 6C g 6C 90 , 120 Monoclinic One 2 or 2 axisc along y a 6C b 6C c; a ¼ g ¼ 90 ; b 6C 90 , 120 Orthorhombic Three mutually perpendicular 2 or 2 axes along x, y, and z a 6C b 6C c; a ¼ b ¼ g ¼ 90 Tetragonal One 4 or 4 axis along z a ¼ b 6C c; a ¼ b ¼ g ¼ 90 Trigonald One 3 axis along z a ¼ b 6C c; a ¼ b ¼ 90 ; g ¼ 120 Hexagonal One 6 or 6 axis along z Cubic Four 3 axes inclined at 54.74 (cosÀ1 1= ﬃﬃﬃ 3 p ) to x, y, and z a ¼ b ¼ c; a ¼ b ¼ g ¼ 90 a We shall see in Chap. 2 that the same relationships apply to conventional unit cells in lattices b The special symbol 6C should be read as “not constrained by symmetry to equal” c It must be remembered that 2 is equivalent to an m plane normal to the 2 axis d For convenience, the trigonal system is referred to hexagonal axes (but see also Table 1.5) Table 1.4 Crystallographic point-group schemea Type Triclinic Monoclinic Trigonal Tetragonal Hexagonal Cubicb R 1 2 3 4 6 23 R 1 m 3 4 6 m3 R + center — 2/m — 4/m 6/m — Orthorhombic R2 222 32 422 622 432 Rm mm2 3m 4mm 6mm Rm — 3m 42m 6m2 43m R2 + center mmm — 4 m mm 6 m mm m3m a The reader should consider the implications of the spaces (marked —) in this table b The cubic system is characterized by its four threefold axes; R refers here to the element 2, 2, 4 or 4, but 3 is always present along h111i 26 1 Crystal Morphology and Crystal Symmetry
- 27. desirable for the purposes of concise and unambiguous communication of crystallographic material. With familiarity, the conventions cease to be a problem. We now consider two point groups in a little more detail in order to elaborate some of the topics discussed so far. Point Group mm2 Once we ﬁx the orientations of two of the symmetry elements in this point group, the third is introduced in a unique orientation. Referring to Fig. 1.28, we start with mm ðm?x and m?yÞ as shown by the thick lines. Point (1), in a general position, is reﬂected across the m plane perpendicular to the x axis (mx) to give point (2). This point is now reﬂected across the second m plane (my) to (3). Then either (3) across mx or (1) across my produces (4). It is evident now that the points in each of the pairs (1), (3) and (2), (4) are related by the twofold rotation axis along z, which is, here, the line of intersection of the two m planes. Point Group 4mm If we start with thefourfold axis along z and m perpendicular to x, we seestraightaway that another m plane (perpendicular to y) is required, Fig. 1.29a, b; the fourfold axis acts on all other symmetry elements in the Table 1.5 Three-dimensional point groups and Hermann–Mauguin notation Symbol meaning for each position System Point groupsa First position Second position Third position Triclinic 1, 1 All directions in crystal – – Monoclinicb 2, m, 2 m 2 and/or 2 along y – – Orthorhombic 222, mm2, mmm 2 and/or 2 along x 2 and/or 2 along y 2 and/or 2 along z Tetragonal 4, 4, 4 m 4 and/or 4 along z – – 422, 4mm, 42m, 4 m mm 4 and/or 4 along z 2 and/or 2 along x, y 2 and/or 2 at 45 to x, y and in xy plane, i.e., along h110i Cubicc 23, m3 2 and/or 2 along x, y, z 3 and/or 3 at 54 440d to x, y, z, i.e., along h111i – 432, 43m, m3m 4 and/or 4 along x, y, z 3 and/or 3 at 54 440d to x, y, z, i.e., along h111i 2 and/or 2 at 45 to x, y, z, i.e., along h110i Hexagonal 6, 6, 6 m 6 and/or 6 along z – – 622, 6mm, 6m2, 6 m mm 6 and/or 6 along z 2 and/or 2 along x, y, u 2 and/or 2 perpendicular to x, y, u and in xy plane Trigonale 3, 3 3 and/or 3 along z – – 32, 3m, 3m 3 and/or 3 along z 2 and/or 2 along x, y, u – a R/m occupies a single position in a point-group symbol because only one direction is involved b In the monoclinic system, the y axis is taken as the unique 2 or 2 axis. Since 2 m, then if 2 is along y, the m plane represented by the same position in the point-group symbol is perpendicular to y. The latter comment applies mutatis mutandis in other crystal systems (it is best to specify the orientation of a plane by that of its normal) c Earlier notation uses m3 and m3m for m3 and m3m, respectively d Actually cosÀ1 ð1= ﬃﬃﬃ 3 p Þ e For convenience; the trigonal system is referred to hexagonal axes; on the axes of a rhombohedral unit cell (q.v.), the orientations of the ﬁrst and second positions of the symbol are [111] and h110i, respectively 1.4 External Symmetry of Crystals 27
- 28. crystalaswell asoncrystalfaces.Ageneralpoint operatedonbythesymmetry4mproduceseightpointsin all, Fig. 1.29c. Thestereogram shows that a second form of (vertical) m planes,lyingat 45 to the ﬁrst set is introduced, Fig. 1.29d. More concisely,we may say that the normals to thetwo forms of m planes lie at 45 to one another. No further points are introduced by the second set of m planes: a fourfold rotation (1) ! (2), followed by reﬂection across the mirror plane normal to the x axis, (2) ! (3), is equivalent toreﬂectionoftheoriginalpointacrossamirrorat45 tox,(1) ! (3).Thereadershouldnowreferagainto Table 1.5 for the relationship between the positions of the symmetry elements and the point-group symbols, particularly for the tetragonal and orthorhombic systems, from which these detailed examples have been drawn. In this discussion, we have used a general form {hkl} to illustrate the point group, and each symmetry-equivalent point lies in a general position, point-group symmetry 1, on the stereogram of the group. The crystal planes that coincide with symmetry planes or symmetry axes are special forms, and their poles lie on symmetry elements: the forms {110} and {010} in 4mm are examples of special forms. The need for the general form in a correct description of a point group is illustrated by Fig. 1.30. The poles of the faces on each of the two stereograms shown are identical, although they may be derived from crystals in different classes, 42m and 4mm in this example (and also in 4 m mm). Figure 1.31 shows crystals of these two classes with the {110} form, among others, developed. In Fig. 1.31b, the presence of only special forms led originally to an incorrect deduction of the point group of this crystal. The stereograms for the 32 crystallographic point groups are shown in Fig. 1.32. The conventional crystallographic axes are drawn once for each system. Two comments on the notation are necessary at this stage. The symbol − + indicates two points, Oþ and , immediately below it and related by a mirror plane in the plane of projection. In the cubic crystal system, the four points related by a fourfold lying axis in the plane of the stereogram lie on a stereographic small circle, which is a circle on the surface of the sphere that does not pass through the center of the sphere, Fig. 1.33. In general, two of the points are projected from the upper hemisphere and the other two points from the lower hemisphere. We can distinguish them readily by remembering that 2 is a subgroup (q.v.) of both 4 and 4. The use of the program SYMM for assisting with point-group recognition is described in Sect. 13.3, and the reader may wish to refer forward at this stage. Appendix B discusses the Sch€onﬂies symmetry Fig. 1.28 Stereogram, symmetry elements, and general form for point group mm2 28 1 Crystal Morphology and Crystal Symmetry
- 29. notation for point groups. Because this notation is also in use in certain contexts, we have written the equivalent Sch€onﬂies symbols in Fig. 1.32, in parentheses, after the Hermann–Mauguin symbols. Subgroups, Laue Groups, Centrosymmetric Groups, and Projection Symmetry Subgroups A subgroup of a given point group is a point group of lower symmetry than the given group, contained within it and capable of separate existence as a point group. For example, 32 is a subgroup of 3m, 622, 6m2, 6 m mm, 432 and m3m, whereas 4 is a subgroup of 4 m , 42m, 4 m mm, 43m, and m3m. The subgroup principle provides a rationale for some of the graphic symbols for symmetry elements. Thus, 4 is shown by a square (fourfold rotation), unshaded (to distinguish it from 4), and with a twofold rotation symbol inscribed (2 is a subgroup of 4). Fig. 1.29 Intersecting symmetry elements. (a) One m plane intersecting the fourfold axis is inconsistent. (b) Consistent group of symmetry elements. (c) General form of points generated by 4m. (d) Complete stereogram, point group 4mm Fig. 1.30 The {110} form in tetragonal point groups. (a) Point group 42m. (b) Point group 4mm 1.4 External Symmetry of Crystals 29
- 30. Laue Groups Point group 1 and point groups that have 1 as a subgroup are centrosymmetric. We shall see later that X-ray diffraction patterns are, in the absence of signiﬁcant anomalous dispersion (q.v.), effectively centrosymmetric, so that the arrangement of spots on the X-ray diffraction photograph of a crystal can exhibit only the symmetry that would be found from a crystal having the corresponding centrosym- metric point group. In the case of a crystal belonging to a non-centrosymmetric point group, the corresponding centrosymmetric point group is simply the given group combined with a center of symmetry. There are 11 such point groups; they are called Laue groups,6 since symmetry is often investigated by the Laue X-ray method, Sect. 5.4.1ff. In Table 1.6, the point groups are classiﬁed according to their Laue group, and the symmetry of the Laue ﬂat-plate ﬁlm photograph is given for directions of the X-ray beam normal to the crystallographic forms listed. Laue-Projection Symmetry The Laue-projection symmetry corresponds to one of the ten two-dimensional points groups. What is the Laue-projection symmetry on {110} for a crystal of point group 4mm? This question can be answered with the stereogram of the corresponding Laue group, 4 m mm. Reference to the appropriate diagram in Fig. 1.32 shows that an X-ray beam traveling normal to {110} encounters 2mm symmetry. The entries in Table 1.6 can be deduced in this way. The reader should refer again to Table 1.5 and compare corresponding entries between Tables 1.5 and 1.6 Fig. 1.31 Tetragonal crystals showing, among others, the {110} form. (a) Copper pyrites, point group 42m. (b) Iodosuccinimide, apparent point group 4mm; X-ray photographs revealed that the true point group is 4 6 Strictly, the term Laue group should be Laue class, but the former is in general use. 30 1 Crystal Morphology and Crystal Symmetry
- 31. Point-Group Projection Symmetry Point-group projection symmetry is the symmetry of the projection of the general form of a point group on to a plane. Thus, the point-group projection symmetry of 4mm on {110} is m. Non-crystallographic Point Groups There are species that exhibit symmetries other than those of the crystallographic point groups. Indeed, R could, in principle, take any integer value between one and inﬁnity. The statement R ¼ 1 implies cylindrical symmetry; the molecule of carbon monoxide has an 1 axis along the C–O bond, if we assume spherical atoms. A ﬁvefold symmetry axis is present in uranium heptaﬂuoride, Fig. 1.34, and the point-group symbol may be written as 10m2, or 5 m m. The stereogram of this point group is shown in Fig. 1.35; the graphic symbol used here for 5 m is not standard. Other examples of non-crystallographic point groups will be encountered among chemical molecules, and a stereogram can always be used to represent the point-group symmetry. In every such example, however, the substance crystallizing in one of the seven crystal systems will normally belong to one of the 32 crystal classes. Fig. 1.32 Stereograms showing both the symmetry elements and the general form {hkl} in the 32 crystallographic point groups. The arrangement is by system and common Laue group. The crystallographic axes are named once for each system and the z axis is chosen normal to the stereogram. The Sch€onﬂies symbols are given in parentheses 1.4 External Symmetry of Crystals 31
- 32. 1.4.3 Quasicrystals, Buckyballs, and Icosahedral Symmetry Quasicrystals Our main task in this chapter has been the description of classical crystallography, in which a crystal is deﬁned as an ideally inﬁnite three-dimensional periodic arrangement of atoms, the periodicities being denoted by the directions of three crystallographic reference axes. Thus, we obtain a crystal structure, with building blocks of atoms (unit cells, q.v.) aligned so as to ﬁll space. Most crystal structures can be described in terms of one of the 230 space groups (q.v.), which show the different types of symmetry elements present in the structures. Until the year 1982, no scientist anywhere would believe in crystals with rotational symmetry degrees other than 1, 2, 3, 4, and 6, as we have discussed earlier: crystals had only these symmetries and were periodic in three dimensions. In that year, however, Professor Daniel Shechtman7 was Fig. 1.32 (continued) 7 Nobel Laureate in Chemistry, 2011. 32 1 Crystal Morphology and Crystal Symmetry
- 33. experimenting with an alloy containing aluminum and manganese, Al6Mn; he was concerned about the appearance of certain areas of the metal surface, Fig. 1.36a, and took a transmission electron micros- copy (TEM) photograph of that region of the surface. He observed diffraction spots in patterns of ten extending over the area of reciprocal space (q.v.) recorded, Fig. 1.36b, and he spent the next 2 years investigating an effect that he found hard to believe. Attempts to explain the results by a process of crystal twinning were unsuccessful, and after more experimentation he was forced to the conclusion of having discovered ﬁvefold symmetry in a crystalline material. The crystal structure is aperiodic: it Fig. 1.32 (continued) 1.4 External Symmetry of Crystals 33
- 34. Fig. 1.33 Stereogram notation for points related by a fourfold axis (y) lying in the plane of a stereogram. The Æ signs refer to the z direction. (a) Vertical section normal to the y axis. (b) Corresponding stereogram; the pairs of points (1)–(2) and (3)–(4) are related by twofold symmetry (subgroup of 4) Table 1.6 Laue groups and Laue-projection symmetry System Point groups Laue group Laue-projection symmetry normal to the given form {100} {010} {010} Triclinic 1, 1 1 1 1 1 Monoclinic 2, m, 2/m 2/m m 2 m Orthorhombic 222, mm2, mmm mmm 2mm 2mm 2mm {001} {100} {110} Tetragonal 4; 4 and 4=m 422; 4mm; 42m; 4 m mm ) 4/m 4 m m 4 m mm 4mm 2mm 2mm {0001} f1010g f1120g Trigonala 3, 3 3 3 1 1 32, 3m, 3m 3m 3m m 2 Hexagonal 6; 6; 6=m 622; 6mm; 6m2; 6 m mm ) 6/m 6 m m 6 m mm 6mm 2mm 2mm {100} {111} {110} Cubic 23, m3 m3 2mm 3 m 432, 43m, m3m m3m 4mm 3m 2mm a Referred to hexagonal axes Fig. 1.34 Stereoview of the molecule of uranium heptaﬂuoride, UF7
- 35. Fig. 1.35 Stereogram of the non-crystallographic point group 10m2 (D5h) showing the general form (20 poles), and a special form of 5 poles lying on the m planes that can be used to represent the ﬁve F atoms in one plane in UF7. The poles for the remaining two F atoms lie at these center of the stereogram, on the 10 axis Fig. 1.36 Transmission electron microscopy (TEM) on an Al6Mn alloy. (a) Surface of the Al6Mn alloy, with irregularities inviting further examination. (b) Copy of Original TEM photograph of the alloy surface taken by Professor Shechtman, showing a tenfold spot pattern indicative of a crystalline nature, but without the periodicity of classical crystals (reproduced by courtesy of Professor Shechtman)
- 36. is space-ﬁlling, but with none of the three-dimensional periodicity that characterizes normal crystals. His ﬁrst paper on these ﬁndings was rejected, but a detailed account was published in 1984 [27]. This alloy structure is denoted a quasicrystal: it has icosahedral symmetry, point group 532; Fig. 1.37 is a simulated Laue pattern for X-ray diffraction from an icosahedral crystal, with the X-ray beam along a ﬁvefold axis. Subsequently, many stable and metastable quasicrystals have been discovered, frequently as binary or ternary intermetallic compounds containing aluminum as one of the constituents. Icosahedral quasicrys- tals form one group of quasicrystals and polygonal quasicrystals, two-dimensional quasicrystals with 8-fold (Mn–Fe–Al), 10-fold (Al–Cu–Ni), or 12-fold (Al–Mn–Si) symmetry yet another. The former group is manifested in the occurrence of sharp diffraction spots and the latter by the presence of a non- crystallographic rotational symmetry. Figure 1.38 is an example of a simulated zero-layer X-ray precession photograph (q.v.) from a polygonal crystal showing 12-fold symmetry (decagonal symmetry) [28]. Two-dimensional quasicrystals symmetry have been reported for rapidly cooled samples corresponding to the compositions V3Ni2 and V15Ni10Si: TEM studies showed that they exhibit 12-fold rotational symmetry but no long-range periodicity [29]. Two-dimensional quasiperiodical structures have been said to occur in medieval mosques and other decorative tilings. Penrose [30] demonstrated the covering of plane space in a non-periodic manner by using two differently shaped units, or tiles, and Fig. 1.39 is an example of a Penrose tiling which shows two superimposed layers of ﬁvefold symmetry. This tiling was extended to three dimensions and, subsequently, a similarity was discovered between Penrose three-dimensional tiling and icosahedral quasicrystals. Mackay has shown experimentally [31] that the diffraction pattern from a Penrose plane tiling has a two-dimensional Fourier transform consisting of sharp d-peaks arranged in a ﬁvefold symmetry pattern. In 2009, naturally occurring quasicrystals were found in Russia [32]; in composition they were Cu–Al–Zn minerals with varying amounts of iron, including an Al63Cu24Fe13 phase; the quasicrystal grains were stated to be of high crystalline quality [33]. Mathematically, the structures of quasicrystals are derivable by a general method that treats them as projections of lattices of higher dimensions. The icosahedral quasicrystals found by Shechtman were shown to be projections from a six-dimensional hypercubic lattice [34]. Whereas three integer Fig. 1.37 Simulated Laue photograph of an icosahedral quasicrystal with the X-ray beam along a ﬁvefold axis (reproduced by courtesy of Dr. Steffen Weber) 36 1 Crystal Morphology and Crystal Symmetry
- 37. values, the Miller indices, are sufﬁcient to label reﬂections in normal crystals, ﬁve linearly indepen- dent vectors are needed for polygonal quasicrystals and six for icosahedral quasicrystals. As a result of the ﬁndings on polygonal crystals and quasicrystals, the International Union of Crystallography revised the deﬁnition of “crystal” as given in Sect. 1.2 to a material capable of producing a clear-cut diffraction pattern, with ordering that is either periodic or aperiodic. The concept of an aperiodic crystal was introduced by Schr€odinger [35]. He sought to explain how hereditary information is stored: molecules were deemed too small, amorphous solids were plainly chaotic, so it had to be a kind of crystal; and as a periodic structure could not encode information, it Fig. 1.39 Example of a Penrose tiling [30] that uses just two shapes of tile (reproduced by courtesy of Jeff Preshing) Fig. 1.38 Simulated zero-layer X-ray precession photograph of a polygonal crystal showing tenfold (decagonal) symmetry (reproduced by courtesy of Dr. Steffen Weber) 1.4 External Symmetry of Crystals 37
- 38. had to be aperiodic. Later, DNA was discovered and, although not crystalline, it possesses proper- ties predicted by Schr€odinger—a regular but aperiodic molecule [36]. In this book, however, the word ‘crystal’ is used in its traditional sense unless otherwise noted. Buckyballs and Icosahedral Symmetry The discovery of a new form of a chemical element is a very rare event, but this occurred with the ﬁnding of a new allotropic form of carbon. Mass spectrometric examination of the products of a high- energy laser interaction with graphite in a helium atmosphere contained fragments with varying numbers of carbon atoms, their distribution depending upon the pressure of helium [37]. A very stable carbon atom cluster was found to be C60. Stability arises because a sheet of carbon atoms formed a ball, thereby satisfying fully the valence requirements of carbon. This situation was met by a structural formation similar to that of a geodesic dome, Fig. 1.40, but with interlocking pentagons and hexagons, and completed to a full sphere, Fig. 1.41. The C60 structure was named buckminsterfullerene [37], after Richard Buckminster Fuller, an American engineer, who described the geodesic dome in detail. The geodesic dome was actually invented in 1922 by Walther Bauersfeld of the Zeiss optical company: it is a spherical or near-spherical lattice- type surface formed by a network of great circles, or geodesics, on a sphere. The geodesics intersect to form a rigid, stress-free triangular structure. Buckminster Fuller developed the mathematics of the dome and popularized it. For simplicity, near-spherical fullerenes are termed buckyballs, the simplest stable structure being buckminsterfullerene [37], C60. This buckyball structure has 32 faces: 20 hexagons and 12 pentagons, Fig. 1.41. Molecules that consist entirely of carbon atoms in the form of hollow spheres, ellipsoids, and tubes are known as fullerenes. Buckyballs and buckytubes are topics of intense research both in pure chemistry, in which fullerenes are manipulated to form compounds, and in technological applications, such as carbon nanotubes. The C60 fullerene exhibits icosahedral symmetry. As icosahedral symmetry is not compatible with translational symmetry, there are no associated crystallographic space groups. Nevertheless, icosa- hedral symmetry can be classiﬁed conveniently under the Sch€onﬂies point group system: full icosahedral symmetry Ih comprises the following symmetry elements: E (identity), C5, C3, C2, i (center of symmetry), S10, S6, s. Thus, the order of the group, the total number of its symmetry elements, is 120. Figure 1.42 illustrates icosahedral symmetry; the similarity to C60 is clear in (b). Fig. 1.40 Example of a geodesic dome (reproduced by courtesy of Lotus Domes UK) 38 1 Crystal Morphology and Crystal Symmetry
- 39. The icosahedral group of lower symmetry I has the elements E, C5, C3, and C2; it is of interest in some biological ﬁelds as it can represent a chiral structure. 1.5 Problems 1.1. The line AC, Fig. P1.1, may be indexed as (12) with respect to the rectangular two-dimensional axes x and y. What are the indices of the same line with respect to the axes x0 and y, where the angle x0 Oy ¼ 120 ? PQ is the parametral line for both sets of axes, and OB/OA ¼ 2. 1.2. Write the Miller indices for planes that make the intercepts given below: (a) a/2, Àb/2, kc. (b) 2a, b/3, c/2. (c) ka, kb, Àc. Fig. 1.42 Icosahedra. (a) Regular icosahedron of vertex ﬁgure 3.3.3.3.3: the vertex ﬁgure means that ﬁve triangles meet at a vertex. (b) Truncated icosahedron of vertex ﬁgure 5.6.6: one pentagon and two hexagons meet at a vertex. The symmetry is Ih in each case Fig. 1.41 Molecular structure of buckminsterfullerene, a C60 buckyball. There are two different bond lengths: 1.458 A˚ for the bonds fusing 5- and 6-membered rings and 1.401 A˚ for bonds fusing the 6-membered rings [38] (Harrison P, McCaw C (2011) Educ Chem 48:113. Reproduced by permission of The Royal Society of Chemistry) 1.5 Problems 39
- 40. (d) a, Àb, 3c/4. (e) ka, Àb/4, c/3. (f) Àa/4, b/2, Àc/3. 1.3. Evaluate zone symbols for the pairs of planes given below: (a) (123), ð011Þ. (b) ð203Þ, (111). (c) ð415Þ, ð110Þ. (d) ð112Þ, (001). 1.4. What are the Miller indices of the plane that lies in both of the zones [123] and ½111? Why are there, apparently, two answers to this problem and to each part of Problem 1.3? 1.5. How many different, unique point groups can be obtained from the symbol 422 by replacing one or more of the rotation axes by roto-inversion axes of the same degree. Write the standard symbols for the unique point groups so derived. 1.6. Take the cover of a matchbox, Fig. P1.2a. (a) Ignore the label, and write down its point group. (b) Squash it diagonally, Fig. P1.2b. What is the point group now? (c) In each case, what is the point group if the label is not ignored? 1.7. Draw stereograms to show the general form in each of the point groups deduced in Problems 1.6a and b. Satisfy yourself that in 1.6a three, and in 1.6b two, symmetry operations carried out in sequence produce a resultant action that is equivalent to another operation in the group. 1.8. How many planes are there in the forms {010}, f110g, and f113g in each of the point groups 2/ m, 42m, and m3? Fig. P1.1 Line referred to rectangular and oblique axes Fig. P1.2 Matchbox: (a) normal; (b) squashed 40 1 Crystal Morphology and Crystal Symmetry
- 41. 1.9. What symmetry would be revealed by the Laue ﬂat-ﬁlm photographs where the X-ray beam is normal to a plane in the form given in each of the examples below? Point group Orientation (a) 1 {100} (b) mm2 {011} (c) m {010} (d) 422 {120} (e) 3 f1010g (f) 3m f1120g (g) 6 {0001} (h) 6m2 {0001} (i) 23 {111} (j) 432 {110} In some examples, it may help to draw stereograms. 1.10. (a) What is the non-trivial symmetry of the ﬁgure obtained by packing a number of equivalent but irregular quadrilaterals in one plane? (b) What is the symmetry of the Dobermann in Fig. P1.3? This example illustrates how one can study symmetry by means of everyday objects. (c) What is the point group of each of the objects in Fig. P1.4a–e, assuming that they all have depth, normal to the plane of the diagram? 1.11. Write the point-group symbol for the species (a) to (v) of molecule or ion in Fig. P1.5, in both the Hermann–Mauguin and Sch€onﬂies notations. Use the program SYMM* with this question for species (a) to (j) and allocate model numbers as follow: (a) 90 (b) 49 (c) 3 (d) 18 (e) 42 (f) 91 (g) 30 (h) 16 (i) 65 (j) 71. Fig. P1.3 Vijentor seal of approval at Valmara, JW 1.5 Problems 41
- 42. 1.12. What is the point-group projection symmetry for each of the examples in Problem 1.9? 1.13. What are the two-dimensional “Miller Indices” (hk) of the lines that form the perimeter of a rectangle? Are they the same for a parallelogram? (Choose appropriate x and y axes with the origin at the center of the ﬁgure.) 1.14. Show from Fig. P1.6 that with Miller–Bravais axes i ¼ Àðh þ kÞ. 1.15. Twelve 1 O resistors are linked to form the edges of a cube, Fig. P1.7. Use the cubic symmetry to determine the effective resistance of the assembly of resistors to a current that is developed by connecting a battery across the ends of a threefold axis. Fig. P1.4 Six symmetrical objects. (a) Dumbbell. (b) Isle of Man style emblem (reproduced by courtesy of Mapsof- World.com). (c) Maltese cross. (d) Flower pattern (reproduced by courtesy of Emeritus Professor John Huffman). (e) Star of David 42 1 Crystal Morphology and Crystal Symmetry
- 43. Fig. P1.5 (a) Carbonate ion; planar. (b) Tetrabromogold(III) ion; planar. (c) Hexachloroplatinum(IV) ion; all Cl–Pt–Cl angles are 90 . (d) Methane all H–C–H angles are 109.47 . (e) Trichloromethane; pyramidal. (f) Bromochloroﬂuoromethane. (g) Benzene; planar. (h) Monochlorobenzene; planar. (i) 1,4-Dichlorobenzene; planar. (j) 1,2-Bromochlorobenzene; planar. (k) Hydrogen peroxide. (l) Orhophosphoric acid. (m) Dibenzyl. (n) Hexanitronickelate(II) ion. (o) Dihydrogen phosphate ion; the hydrogen atoms are arranged statistically on the four positions shown. (p) 1,2,4,-Trichlorobenzene; planar. (q) 2,4,6-Triazidotriazine; planar. (r) trans-1,2-Dichlo- roethane; planar. (s) Cycloocta-1,5-diene. (t) Tetranitrodiamminocobaltate(III) ion. (u) Pentaﬂuoroantimonate(III) ion. (v) Thorium tetrabromide 1.5 Problems 43
- 44. Fig. P1.5 (continued) 44 1 Crystal Morphology and Crystal Symmetry
- 45. Fig. P1.5 (continued) 1.5 Problems 45
- 46. Fig. P1.5 (continued) 46 1 Crystal Morphology and Crystal Symmetry
- 47. Fig. P1.5 (continued) 1.5 Problems 47
- 48. Fig. P1.5 (continued) 48 1 Crystal Morphology and Crystal Symmetry
- 49. References and Bibliography 1. Exodus 28:17–20; Revelation 21:19–20 2. Gessner C (1564) De rerum Fossilium, Lapidum et Gemmarum, Figuris. Z€urich 3. Pliny the Elder (77–79) Naturis historiæ. Rome 4. Caesalpinus A (1596) De metallicis libri tres. Rome Fig. P1.6 Equivalence of i and À(h þ k) with Miller–Bravais axes Fig. P1.7 The cube shown consists of twelve 1 O resistors; the current I follows a path from A to G References and Bibliography 49
- 50. 5. Buffon G-LL (1807) Buffon’s natural history. London 6. Stensen N (Steno N) (1669) De solido intra solidum naturaliter contento dissertationis prodromus, book 3. Florence 7. Bartholinus E (1669) Experimenta Crystallici Islandici. Copenhagen 8. Kepler J (1611) Strena Seu de Nive Sexangula. Frankfurt 9. Guglielmini D (1688) Riﬂessioni ﬁlosoﬁche dedotte dalle ﬁgure de Sali. Bologna 10. Rome´ de l’Isle J-BL (1783) Cristallographie. Paris 11. Carangeot A (1782) Nouvelles de la Re`publique des lettres et des arts, no. 14. Paris 12. Ha€uy RJ (Abbe´ Ha€uy) (1801) Traite´ e´le´mentaire de physique. Paris 13. Weiss CS (1815) Abhandlungen, der K€oniglichen Akademie der Wissenschaften. Berlin 14. Mohs F (1822) Grund-Rib der Mineralogie. Dresden 15. Hessel JFC (1830) Kristall. Gehlers Physikalische W€orterbuch. Leipzig 16. Frankenheim ML (1842) Nova Acta Acad, vol 19. von Grass, Breslau 17. Miller WH (1839) Treatise on crystallography. Cambridge 18. Bravais A (1846) Mem Acad R Sci Inst France 9:255 19. Federov Y (1891) Zap Mineral Obch 28:1 20. Sch€onﬂies A (1891) Kristallsysteme und Kristallstruktur. Leipzig 21. Barlow W (1894) Z Kristallogr 23:1 22. Freidrich W, Knipping P, Laue M (1912) M€unchener Ber:303; (1913) Ann Phys 41:917 23. Bragg WL (1913) Camb Philos Soc 17:43 24. Bragg WH (1913) Proc R Soc 88A:428 25. Carlisle CH, Ladd MFC (1966) Acta Crystallogr 21:689 25a. http://proteopedia.org/wiki/index.php/Nobel_Prizes _for_3D_Molecular_Structure 26. Plato (1955) The republic, book VII, circa 360 B. C. E. (trans: Lee HDP). Penguin Books, Harmondsworth 27. Shechtman D et al (1984) Phys Rev Lett 53:1951 28. €Unal BV et al (2007) Phys Rev B 75:064205 29. Chen H et al (1988) Phys Rev Lett 60:1645 30. Penrose R (1976) Sets of tiles for covering a surface. US Patent 413315 31. Mackay AL (1982) Physica A114:609 32. Bindi L et al (2009) Science 324:1306 33. Steinhardt P et al (2011) Philos Mag 91:2421 34. Kramer P et al (1984) Acta Crystallogr A40:580 35. Schr€odinger E (1944) What is life. Cambridge University Press, Cambridge 36. http://tc.engr.wisc.edu/uer/uer96/author9/index.html 37. Kroto H et al (1985) Nature 318:162 38. Hedberg K et al (1991) Science 254:410 Bibliography: General and Historical Study of Crystallography Bragg WL (1949) A general survey, vol I, The crystalline state. Bell, London Ewald PP (ed) (1962) Fifty years of X-ray diffraction. Oosthoek, Utrecht Hauptmann HA (1990) Structural chemistry, vol 1. Springer, New York Lonsdale K (1948) Crystals and X-rays. Bell, London Crystal Morphology and Stereographic Projection Phillips FC (1971) An introduction to crystallography. Longmans, London Crystal Symmetry and Point Groups Hahn T (ed) (2002) International tables for crystallography, vol A, 5th edn. Kluwer Academic, Dordrecht Henry NFM, Lonsdale K (eds) (1965) International tables for X-ray crystallography, vol I. Kynoch Press, Birmingham. http//:it.iucr.org Ladd MFC (1989) Symmetry in molecules and crystals. Ellis Horwood, Chichester Ladd Mark (1998) Symmetry and group theory in chemistry. Horwood Publishing, Chichester 50 1 Crystal Morphology and Crystal Symmetry

No public clipboards found for this slide

×
### Recorte os slides mais importantes para salvá-los

Recorte slides de uma apresentação para colecionar e organizá-los de forma eficiente. Inclua seus slides favoritos em um painel de recortes para classficá-los de acordo com tópico.

Looks like you've clipped this slide to already.

Criar um painel de recortes

Be the first to comment